1 Technical Notes 6 - Painting Brick Masonry Rev [May 1972] (Reissued December 1985) INTRODUCTION Although some masonry walls require protective coatings to impart color and help in resisting rain penetration, clay masonry requires no painting or surface treatment. Brick are generally selected because, among other characteristics, they have integral and durable color and, when properly constructed, are resistant to rain penetration. Clay masonry walls may be painted to increase light reflection or for decorative purposes. Most paint authorities agree that, once painted, exterior masonry will require repainting every three to five years. This issue of Technical Notes discusses general applications of paint to interior and exterior brick walls, and a brief discussion on specific paints suitable for brick masonry. GENERAL It is often erroneously assumed that brick masonry walls that are to be painted can be built with less durable materials and, in some instances, with less than extreme care in workmanship than would normally be used for unpainted brick walls. This is not the case. When a brick wall is to be painted, the selection of materials, both brick units and mortar, and the workmanship used in constructing the wall should all be of the highest quality; at least as good in quality as when the walls are to be left exposed. Every care should be taken to see that joints are properly filled with mortar to avoid the entrance of moisture into the wall, since it may become trapped behind the paint and cause problems. Every care should be taken to see that there are no efflorescing materials in the wall, either in the mortar, brick units or in the backup, since efflorescence beneath the paint film can also cause problems. See Technical Notes 23 Series. Brick. Brick units to be used for walls that are to be painted should conform to the applicable requirements of the ASTM Specifications for Building Brick or Facing Brick, C 62 or C 216, respectively. The grade of units (which designates their durability) should not be lower than would be used if the wall were not to be painted. Grade SW is recommended. It may be acceptable to use brick units which are durable but differ in color in a wall to be painted. However, care should be taken that the units have similar absorption and suction characteristics so that the paint applied will adhere to all of the surfaces and have a uniform acceptable appearance. Mortar. Mortar for brick masonry walls to be painted should conform to the Specifications for Mortar for Unit Masonry, ASTM C 270, Proportion Specifications. It is suggested that the mortar consist of portland cement and lime, and that the mortar type be selected on the basis of the structural requirements of the wall. See Technical Notes 8. Paint. Paint for application to brick masonry walls should be durable, easy to apply and have good adhesive characteristics. It should be porous if applied on exterior masonry, thereby permitting the wall to breathe and preventing the trapping of free moisture behind the paint film. CONSIDERATIONS FOR PAINTING CLAY MASONRY In selecting a paint system for a brick masonry wall, the primary concern should be the characteristics of the surface and the exposure conditions of the wall. A primer coat may be of particular importance, especially where unusual or severe conditions exist.
2 Alkalinity. The chemical property of masonry which may have a significant effect on paint durability and performance is the alkalinity of the wall. Brick are normally neutral, but are set in mortars which are chemically basic. Paint products, which are based on drying oils, may be attacked by free alkali and the oils can become saponified. To prevent this occurrence, an alkaline-resistant primer is recommended. Efflorescence. The deposit of water-soluble salts on the surface of masonry, efflorescence, is another factor that can hamper the performance of painted masonry. Efflorescence, which is present on the surface, should be removed and, once removed, the surface should be observed for reoccurrence prior to being painted. Methods of preventing and removing efflorescence are discussed in Technical Notes 23 Series, "Efflorescence-Causes, Prevention and Control". Water and Moisture. Water or moisture in a masonry system will generally hamper the satisfactory performance of the painted surface. Moisture may enter masonry walls in any of several ways; through the pores of the material, through incompletely bonded or only partially filled mortar joints, copings, sills and projections, through incomplete caulked joints and improperly installed flashing or where flashing is omitted. In general, brick wall surfaces should be dry for painting. Acceptable moisture conditions for masonry walls to receive paint are listed in Table 1. The use of an electrical moisture meter may be used to measure the moisture content of a wall 1 Some manufacturers offer special porous, highly pigmented emulsion paints which may give somewhat better results in very adverse conditions where delay is not acceptable. SURFACE PREPARATION General. Proper surface preparation is as important as paint selection. Because each coat is the foundation for all future coats, success or failure depends largely upon surface preparation. Thoroughly examine all surfaces to determine the required preparation. Previously painted surfaces often require the greatest effort. Before painting, remove all loose matter. Take special care when cleaning surfaces for emulsion paints and primers. They are nonpenetrating and require cleaner surfaces than solvent-based paints. Some paints can or should be applied to damp surfaces. Others must not. Be sure to follow directions accompanying proprietary brands. New Masonry. As a general rule, new clay masonry is seldom painted. It is difficult to justify the extra expenditure for initial and future painting. However, if for any reason painting new masonry is desired, there are a few precautions necessary for reasonable success. Do not wash new clay masonry walls with acid cleaning solutions. Acid reactions can result in paint failures. Use alkali-resistant paints. If low-alkali portland cement is not used in the mortar, it may be necessary to neutralize the
3 wall to reduce the possibility of alkali-caused failures. Zinc chloride or zinc sulfate solution, 2 to 3 1/2 lb per gal of water, is often used for this purpose. Existing Masonry. Examine older unpainted masonry for evidence of efflorescence, mildew, mold and moss. While these conditions are not common, they all indicate the presence of moisture. Examine all possible entry points for water. Where necessary, repair flashing and caulking; tuckpoint defective mortar joints. Remove all efflorescence by scrubbing with clear water and a stiff brush. A wall which has effloresced for a long time may present difficulties. The presence of moisture, the deposition of salts and the probable presence of alkalies are all factors which may contribute to the deterioration of paints. If moss has accumulated on damp, shaded masonry, apply an ordinary weed killer. Wet the wall with clear water before applying weed killers to prevent them from being drawn into the wall. Chemical weed killers may contain solubles which can contribute to efflorescence or react unfavorably with paint, and should be removed after being used by scrubbing the wall with a stiff brush while rinsing with clear water. Mildew seldom occurs on unpainted masonry. However, where present, treat it the same as on painted surfaces, discussed in the following paragraphs. Be sure to wet the wall before applying any cleaning solution. Clean small areas and rinse thoroughly. For further discussion on cleaning brick see Technical Notes 20 Revised, "Cleaning Clay Products Masonry". Painted Surfaces. Previously painted surfaces normally require extensive preparation prior to repainting (refer to Table 2 for typical paint failures). Under humid conditions, mildew may have developed. Mildew may feed on a paint film or on particles trapped by the painted surface. If present, remove it completely before applying paint. Otherwise, growth will continue, damaging new paint. Mildew has been successfully removed by steam cleaning and sand blasting. The following is also effective: 3 oz trisodium phosphate (Soilax, Spic and Span, etc.), plus 1 oz detergent (Tide, All, etc.), plus 1 qt 5 per cent sodium hyperchlorite (Chlorox, Purex, etc.), plus 3 qt warm water, or enough to make 1 gal of solution. Use this solution to remove mildew and dirt. Scrub with a medium soft brush until the surface is clean; then rinse thoroughly with fresh water. For small areas, use an ordinary household cleanser. Scrub with a medium soft brush and then rinse thoroughly. Use masonry paints containing a mildewcide to help prevent molds from recurring. Remove all peeled, cracked, flaked or blistered paint by scraping, wire brushing or sand blasting. In some instances, old paint may be burned off, but this should be done only by skilled operators. Like efflorescence, paint blistering is caused by water within the masonry. Search for the water's source and take the necessary corrective measures to keep water out of the wall. If alligatoring exists, remove the entire finish. There is no other means of correction. If slight chalking has occurred, brush the surface thoroughly. However, if chalking is deep, remove by scrubbing with a stiff fiber brush and a solution of trisodium phosphate and water. Rinse the surface thoroughly afterwards. Use a penetrating primer to improve adhesion of the final coat. Excessive paint buildup results from too many coats or excessively thick coats. Where it occurs, remove all paint and treat as a new surface. Completely remove cement-based paints before repainting with other types. An exception to this rule is the use of cement-based paints as primers which will be covered by another paint within a relatively short time. If the wall will be repainted with another cement-based paint, wire brushing and scrubbing will suffice, providing treatments for mildew, efflorescence, etc. are not required.
4 TABLE 2 Types of Paint Failure MASONRY PAINTS Because all paints have distinct properties and because surfaces vary considerably, even the most experienced painting contractors carefully examine a surface before making recommendations. However, the following will generally indicate the proper use of masonry paints. CEMENT-BASED PAINTS For many years, cement-based paints have been satisfactory coatings for masonry surfaces. They achieved popularity because they have relatively good adherence and tendency to make a wall less permeable to free water. Cement-based paints are permeable, permitting the wall to breathe. Their main components are portland cement, lime and pigments. Additives, binders and sands may be added. Although cement-based paints are more difficult to apply than other types, good surface protection results when properly applied. While they are not complete waterproofers, cement-based paints help to seal and fill porous areas, excluding large amounts of free water. White and light colors tend to be the most satisfactory. It is difficult to obtain a uniform coating with darker shades. Lighter colors tend to become translucent when wet, and dark colors become darker. Color returns to normal as the wall surface dries. Cement-based paints can provide a good base for other paints applied within a relatively short time. The following procedure for applying paint on a properly prepared surface generally applies: 1. Cure new masonry walls for approximately one month before applying cement-based paints. 2. Dampen wall surfaces thoroughly by spraying with water. 3. Cement-based paints are packaged in powdered form. Because their cementitious components begin to hydrate upon contact with water, mix immediately prior to application for optimum results. 4. Apply heavy coats with a stiff brush, allowing at least 24 hr to elapse between coats.
5 5. During this time, keep the wall damp by periodically spraying it with water. 6. Apply additional coats in the same manner. 7. Keep the final coat damp for several days to properly cure. WATER-THINNED EMULSION PAINTS General Characteristics. Water-thinned emulsion paints, commonly referred to as latex paints, are relatively easy to apply. Water-thinned emulsions may be brush, roller or spray-applied. However, brush application is preferable, especially on coarse-textured masonry. Emulsion paints dry quickly, have practically no odor and present no fire hazard. They may be applied to damp surfaces, permitting painting shortly after a rain or on walls damp with condensation. As a group, these paints are alkali-resistant. Hence, neutralizing washes and curing periods are not usually necessary before painting. Water emulsion paints possess high water vapor permeability and are known to have performed well on brick substrates that have been properly prepared. Emulsion paints will not adhere well to moderately chalky surfaces. If possible, repainting should be done before the previous coat chalks excessively. However, specifically formulated latex paints are available containing emulsified oils or emulsified alkyds which facilitate wetting of chalky surfaces. This property enables the paint to bond the chalk together and to the substrate. The principal water-thinned emulsion paint types are: butadiene-styrene, vinyl, acrylic, alkyd and multicolored lacquers. Butadiene-Styrene Paints. These relatively low-cost, rubber-based latex paints develop water resistance more slowly than vinyl or acrylic emulsions. They are most satisfactory in light tints as chalking rate may be excessive in deep colors. Vinyl Paints. Polyvinyl acetate emulsion paints dry faster, have improved color retention and a more uniform, lower sheen than rubber-based latex paints. Acrylic Emulsion Paints. Acrylic emulsions have excellent color retention, permit recoating in 30 min or less, and have good alkali resistance. Acrylics have high resistance to water spotting and may be scrubbed easily. Alkyd Emulsion Paints. Alkyd emulsions are related to solvent-thinned alkyd types, but have all the general characteristics of latex paints. They do have more penetration than most water-thinned emulsions, achieving better adhesion on chalky surfaces. Compared to other emulsion paints, these are rather slow to dry, have more odor, are not as resistant to alkalies, and have poorer color retention. Under normal exposure conditions, alkyd emulsions can serve as a finished coat over a suitable primer. Multicolored Lacquers. A specialized paint group, multicolored lacquers are applied only by spray gun. The finished film appears as a base color with separate dots or particles of contrasting colors. These paints will cover many surface defects and irregularities. However, they must be applied over a base coat of another type; for example, polyvinyl acetate or acrylic emulsion paints. FILL COATS Fill coats are base coats for exterior masonry. They are similar in composition, application and uses to cementbased paints. However, fill coats contain an emulsion paint in place of some water, giving improved adhesion and a tougher film than unmodified cement paints. Fill coats have greater water retention, giving the cement a better chance to cure. This is particularly valuable in arid areas where it is difficult to keep the painted surface moist during the curing period. SOLVENT-THINNED PAINTS The five major solvent-thinned paints are oil-based, alkyd (synthetic resin), synthetic rubber, chlorinated rubber and epoxy. Oil-based and alkyd paints are not recommended for exterior masonry. Solvent-thinned paints should
6 be applied only to completely dry, clean surfaces. They produce relatively nonporous films and should be used only on interior masonry walls not susceptible to moisture penetration. The exception to this is special purpose paint, such as synthetic rubber, chlorinated rubber and epoxy paints. Oil-Based Paints. Oil-based paints have been used for many years. They are relatively non-porous and recommended for interior use only. Although several coats may be required for uniform color and good appearance, they bind well to porous masonry. As with most solvent-based paints, they have good penetration on relatively chalky surfaces, but are highly susceptible to alkalies. New masonry must be thoroughly neutralized to avoid saponification. Available in a wide color range, oil-based paints are moderately easy to apply. Several days' drying is generally required between coats. Alkyd Paints. Alkyd paints are similar to oil-based paints in most general characteristics. They may have slightly less penetration, resulting in somewhat better color uniformity at the cost of adhering power. Alkyd paints are more difficult to brush, dry faster and give a harder film than oil-based paints. These, too, are nonpermeable and are recommended for interior use only. Synthetic Rubber and Chlorinated Rubber Paints. These paints have excellent penetration and good adhesion to previously painted, moderately chalky surfaces as well as new surfaces. They are reported to be more resistant to efflorescence and are generally good in alkali resistance. They may be applied directly to alkaline masonry surfaces, but are more difficult to brush on than oil paints. Darker colored synthetic rubber paints lack color uniformity. Both types have high resistance to corrosive fumes and chemicals. For this reason, they are often specified for industrial applications. Both types require very strong volatile solvents, a fire hazard which may prove undesirable. Epoxy Paints. Epoxy paints are of synthetic resins generally composed of two parts, a resin base and a liquid activator. They must be used within a relatively short time after mixing. Epoxies can be applied over alkaline surfaces, have very good adhering power, and good corrosion and fume resistance. However, some types chalk excessively if used outdoors. Epoxies are relatively expensive and somewhat difficult to apply. "HIGH-BUILD" PAINT COATINGS High-build paint coatings are generally used on interiors to give the effect of glazed brick. Some coatings are based on two-component urethane polyesters and epoxies. Others are of an emulsion-based coat with acrylic lacquer. These paint systems usually include fillers to smooth out surface irregularities. OTHER COATINGS Heavily applied coatings of the so-called "breathing type" are available with either a water or solvent base. They are generally composed of asbestos fiber and sand, and applied thickly to hide minor surface imperfections. The presence of moisture on the surface of a masonry wall generally will not harm the latex type. Lower application temperatures of 35 F to 50 F on the other hand are less damaging to the solvent type. For both types, adhesion is mostly mechanical because of low binder and high pigment content. Some coatings require special primers to insure adhesion. Although these coatings are reported to have given good performance on masonry, they tend to show stains where water runoff occurs. These coatings are capable of allowing passage of water vapor, but cannot transmit large quantities of water that may enter through construction defects. Failure may occur as a result of freezing of water accumulation behind the film. PAINTING NEAR UNPAINTED MASONRY Often windows and trim of masonry buildings are painted with self-cleaning paints to keep surfaces fresh and clean. Unfortunately, self-cleaning is generally achieved through chalking. The theory is that rain will wash away chalked paint, constantly exposing a fresh paint surface. The theory works well, but too often no provision is made to keep chalk-contaminated rain water away from masonry surfaces. The result is usually more unsightly than dirty paint on trim or windows. Avoid this staining by choosing nonchalking paints for windows and trim and by providing a means of draining water away from wall surfaces.
7 REFERENCES 1. Manual on the Selection and Use of Paints, Technical Report #6, National Research Council of Canada, Division of Building Research, 1950, Ottawa, Canada. 2. Paints for Exterior Masonry Walls, BMS110, National Bureau of Standards, 1947, Washington, D.C. 3. Field Applied Paints and Coatings, Publication 653, Building Research Institute, 1959, Washington, D.C. 4. Paints and Coatings, Publication 706, Building Research Institute, 1960, Washington, D.C. 5. Painting Walls; 1, Building Research Station Digest (2nd Series), No. 55, Building Research Station, 1965, Garston, Herts., England. 6. Coatings for Masonry Surfaces, by H. E. Ashton, Canadian Building Digest, CBD 131, November 1970, Ottawa, Canada. 7. Coatings for Masonry and Cementitious Materials, by Walter Bayer, Construction Specifier, November
Stage 3: Fixing/Pre-Paint Stage Information on Painting The First Coat of Paint is the Most Important Most project homes are specified with a 2 coat finish. Master Painters of Australia recommends 3 coats,
Guide to Waterproofing Solutions for interior and exterior use Excessive moisture in basements and foundation walls can cause significant problems including structural decay, high humidity levels and mold
extension.usu.edu Smart Shopping for Home Furnishings Selecting Paint Dr. Leona Hawks Home Furnishings & Housing Specialist 1987 HI 13 Shopping for paint? When shopping for paint, you will find many different
How to Paint your Pool Introduction Painting is one of the best ways to protect and beautify your pool. In addition to adding a vibrant, fresh color, a new coat of paint can be a cost- efficient way to
Installation manual for Authentic Stone Veneer Please read carefully before installing: Install all Authentic Stone Veneer in accordance with ACI 530.1/ASCE 6/TMS 602 Specifications for Masonry Structures.
HSTOPS A WALL OF WATER 22 FT. HIG! F U L LY T R A N S F E R A B L E RESISTS10 PSI ! 1 F U L LY T R A N S F E R A B L E HSTOPS A WALL OF WATER 22 FT. HIG RESISTS10 PSI Guaranteed To Stop Water Even Under
LIME RENDER & WHY BUILDINGS NEED TO BREATHE KEIM MINERAL PAINTS THE NEED FOR BUILDINGS TO BREATHE Before the twentieth century, building techniques and materials were very different from those used today
Cleaning of Clay Brickwork Maintenance & Repair. No 4.1 December 2001 INTRODUCTION This publication describes techniques which may be used for the cleaning of newly built brickwork, the surface of which
Application of Exterior Wood Finishes The following information is excerpted from the publication, Exterior Wood in the South Selection, Applications, and Finishes by Daniel L. Cassens and William C. Feist;
Overview 0 Paint & Body Defects is one of the 3 most consistent indicators when inspecting for prior repairs that could ultimately indicate structural repairs, existing damage or alterations. 0 Use this
cement Masonry Cement Engineered for quality and reliability, Lafarge cements for masonry deliver consistent performance. page 2 Lafarge Cement Lafarge in North America The Lafarge Group is the world leader
New Football Stadium 09.91.13-1 PART 1 GENERAL 1.01 SECTION INCLUDES A. Surface preparation. B. Field application of paints. SECTION 09.91.13 EXTERIOR PAINTING C. Scope: Finish exterior surfaces exposed
Tel: 404 346-3666 Toll Free: 800 221-2397 Fax: 404 346-3119 Stucco Repair and Maintenance No. 1.01 These stucco repair and maintenance techniques are intended as a partial guide to repair of stucco walls.
Keeping your tractor or equipment well kept & free from rust & corrosion will extend the life of your investment & help retain its value for a longer period of time. It can be difficult, in many cases,
Cracks, chips and broken or flaking areas in concrete are not only unsightly, they can lead to further deterioration of the surface. The result is a costly replacement project as opposed to a simple repair.
BARN & FENCE PAINT NO. 25 BARN RED Smooth or rough sawn exterior vertical wood surfaces such as plywood, fences, shingles, shakes, siding. laminates, masonry and stucco surfaces. AVAILABLE IN: Gallon Only
Application Guide Type EP Epoxy Overview Supplies Needed Ramuc Type EP Epoxy offers a hard, tough, durable finish, providing stain, chemical, and abrasion resistance for protection of concrete, plaster,
A bout your HOUSE before you start Repairing And Replacing Materials Exterior Walls CE 28 h Exterior finish materials are expected to protect the house from the elements while providing an attractive appearance.
INDUSTRIAL FLOORING INSTALLATION CHALLENGES James C. Ziegler, ArmorSeal Product Manager Sherwin Williams Cincinnati, Ohio, USA Abstract: Specifier's and contractors not only need to properly evaluate the
Section 099100 Painting and Finishes (General) PART 1 - GENERAL 1.01 Conditions A. The general provisions of the Contract, including General Conditions and Special Provisions apply to the work specified
Application Instructions for Keystone Kool Deck on Existing Concrete REQUIRED MATERIALS Keystone Kool Deck PTA Bonding Agent Water 20 Mesh Marble Sand White Portland Cement OPTIONAL TOOLS Mortex Ad-Tex
PRE-TREATMENT MATERIALS KEIM MINERAL PAINTS PRE-TREATMENT When decorating surfaces, effective pretreatment will significantly extend the longevity and protection of the painted system. This is particularly
Technical Information White rust on galvanised steel Prevention It is easier to prevent white rust than to cure it! Reasonable precautions to protect steel during both transport and storage can considerably
General Surface Preparation Proper surface preparation will contribute significantly to the longevity of Ace Paint products. Follow these general guidelines for best results. CLEAN: Paint will not adhere
Patrick Loughran, AIA, PE, LEED AP July 13, 2007 Page 1 Efflorescence in Masonry: Understanding the Problems and Solutions By Patrick Loughran, AIA, PE, LEED AP Reprinted by permission of the author. The
TOPCOAT Liquid-Applied Roofing Systems TOPCOAT System Specifications EPDM (TOPGN160) Updated: 7/14 TOPCOAT System Specifications EPDM PART 1 GENERAL 1.01 SYSTEM DESCRIPTION U.S. Only The TOPCOAT Roofing
Selection and Use of Coatings, Water Repellents, and Sealants to Control Moisture Intrusion in Above-Ground Concrete and Masonry Walls Kenneth A. Trimber KTA-Tator, Inc. Coating, Water Repellent, Sealant
Fixing Instructions: 01 Porcelain to Screeded Concrete Floors Surface Tiles can be fixed to all structurally sound surfaces consisting of concrete, sand and cement screeds and renders, blockwork, masonry,
PAGE: 1 of 6 PRINT DATE: 16/09/2004 BLACK JACK ALL WEATHER ROOF COATING DESCRIPTION BLACK JACK ALL WEATHER ROOF COATING is a solvent based, full bodied black brushable compound with added fibres for reinforcement.
Acrylic Enamel Topcoat ACRYL-GLO TECHNICAL DATA SHEET The ACRYL-GLO single-stage acrylic enamel paint system provides a durable finish that is easy to apply and suitable for both commercial and passenger
Stone Developments Irish Blue Limestone Maintenance Guide Caring for Irish Blue Limestone Products As an naturally occurring material, blue limestone is ideally suited to withstand environmental stresses,
Product Data 408 Epotec Primer Surfacer PRODUCTS Epotec Primer Surfacer Epotec Primer Hardener Thinners 408-Pack A 414-9105 Pack B R202-Normal conditions, R270-Hot conditions Product Description A polyamide
Acrylic Coatings: The Perfect Stucco Finish By Larry Miller and Joe Miller Whether a stucco surface is new or old, there are many different finish coatings in today s marketplace that are supposedly right
ONBOARD MAINTENANCE PAINT GUIDE CONTENT Page A practical Onboard Maintenance Paint Guide 1.0 2.0 3.0 INSPECTION AND PLANNING 4 HSE 6 SURFACE PREPARATION 8 The purpose of this guide is to provide easy and
CROWN PAINTING SCHEDULE ALL PAINTS AVAILABLE THROUGH SHERWIN-WILLIAMS PAINT STORES. PLEASE GO TO sherwinwilliams.com store locator to find the store closest to you. These paints are mainly commercial/industrial
8 chapter External solid plastering OVERVIEW Render provides a weatherproof surface that prevents the penetration of moisture into the outside of the building, and forms a decorative finish that enhances
"YOUR OLD HOUSE" - Paint By Ken Marchtaler, Certified Coatings Consultant Your Heritage Paint Project The materials used in constructing heritage buildings are often considered well above the standards
07560 BUR BUILT-UP ROOF COATING SMOOTH and GRANULE SURFACE SPECIFICATION PART 1: GENERAL 1.01 SCOPE: To extend the useful service life of the aged or new asphalt built-up roof system and to reduce cooling
Elastomeric Masonry, Stucco & Brick Paint For Exterior Use 100% Acrylic Latex Stretches up to 600% to Resist Cracking Formulated with a Mildewcide Low Sheen No. 68 White Properly prepared exterior vertical
Part 1 General 1.1 Summary.1 Unless otherwise indicated, follow the standards below when specifying re-painting. These standards are not intended to restrict or replace professional judgment..2 This Section
RECOATING AND RENEWING SPF ROOFING SYSTEMS Procedures, Regional Differences and type of coating systems Bruce Schenke Premium Spray Products REASONS TO RECOAT/RENEW Add a new coating layer to renew the
Maintenance Guide Heveatech Decking Table of Content Introduction 3 Daily Cleaning 4 Removing Mold 5 Recoating 6 Introduction Once you have decided to invest in a decking with Heveatech, there are some
A quick reference guide to Effective Waterproofing Identifying Damp The term damp strikes fear into the hearts of most homeowners. Left untreated, a small, easily repairable problem can become much larger
Commercial Luxury Vinyl Tile Installation System Product Gauge Size Adhesive NATURAL CREATIONS 0.125" (3.2 mm) Various Sizes and Shapes S-288, S-543*, or S-240** * It is necessary to smooth out the adhesive
SECTION 099123 - INTERIOR PAINTING PART 1 - GENERAL 1.1 RELATED DOCUMENTS A. Drawings and general provisions of the Contract, including General and Supplementary Conditions and Division 01 Specification
DIVISION 8 PAINTING SPECIFICATIONS 8.1 General 8.1.1 Scope Contractor shall provide all labor, material, and equipment and perform all operations necessary for all painting work specified including the
INSTALLATION OF ECOWORX MODULAR CARPET INSTALLATION GUIDELINES THE FOLLOWING INSTRUCTIONS SHOULD BE REVIEWED PRIOR TO INSTALLATION AS WELL AS MEETING THE REQUIREMENTS OF AS2455.1:2007 & AS2455.2:2007 (WHERE
Wonder Wood Stain (WWS) Exterior Stain Product Overview Sales Version Wonder Wood Stain Waterborne Exterior Semi-Transparent Stain What does the professional stain contractor look for in a stain? No problems
Epoxy/Urethane Concrete Coating System Application Guide Endura offers a coating system for concrete floors consisting of an epoxy primer and a urethane topcoat. It can be used on garage, warehouse and
1/5 pages Systems 3 coats Cetol HLSe or 1 coat Cetol HLSe and 2 Coats Cetol Deck or 1 coat Cetol HLSe and 2 Coats Cetol Deck plus Please select required system. Key Practical coverage in m²/ltr per coat,
INFUSION REACTIVE STAIN systems guide Helping you protect, restore and beautify your concrete Create UNique DESIGNS NEVER TO BE DUPLICATED H&C *VOC INFORMATION H&C INFUSION Reactive Concrete Stain, Water
WARRANTY INFORMATION: SPECIAL PAINTING REQUIREMENTS: The warranty for this product shall be void if the Product sections are not painted or sealed in accordance with DASMA TDS 162 (available at www.dasma.com)
Table of Contents: Page: Troubleshooting Issue: 2. Color Differential 3. Fish Eye 4. Milky or Cloudy Coatings 5. Orange Peel 6. Peeling or Delamination 8. Delamination between Coats 9. Pinholes/Bubbling
Installing Tile in Pools and Fountains Waterproofing, Surface Preparation and Thin-set Mortar Selection are Critical Steps in Submerged Tile Projects. By Steve Taylor, Director of Architecture and Technical
EPOXY-RESIN TERRAZZO FLOORING GENERAL INFORMATION 1.1 Epoxy-resin thin-set terrazzo flooring installed on concrete subfloors. 1.2 Comply with the recommendations of the National Terrazzo and Mosaic Association
INTRODUCTION WHAT IS K2 NATURAL THINSTONE VENEER? Natural K2 Stone veneer is real stone, cut 1 inch thick, making it light enough to be installed as a veneer. Sometimes referred to as thin veneer, thin
COLOR & COATING GUIDE >> A complete selection guide of Johnson Controls finishes COLOR GUIDE AVAILABLE FINISH COLORS POLYESTER POWDER COAT #81 PALE BROWN #83 CHOCOLATE BROWN #85 TIMELESS BRONZE #70 BLACK
4. Preparatory Work 4.1 PLANNING Quality control starts with good planning and management. An Inspection and Test Plan, ITP (refer to Appendix D) which lists down the project s inspection and testing requirements
Selecting Sealants Based on Masonry Movement The Construction Specifier August 2002 Movement capability must be considered when selecting the proper sealant for joints in clay or concrete masonry walls.
PUTTY & POWDER 17 18 Nano Wall Putty DESCRIPTION: Nanotechnology based Nano Filler (Wall Putty) is complete water based material that is durable, water repellent, crack resistant, UV resistant, fungus/
TECHNICAL INFORMATION CES-311 10/12 SUPERSEDES 01/03 PAGE 1 OF 7 CORROSION ENGINEERING SPECIFICATION FOR INSTALLATION TUFCHEM TILING SYSTEMS 1. SCOPE 1.1 Corrosion-resistant tile flooring is broadly used
SECTION 099113 - EXTERIOR PAINTING PART 1 - GENERAL 1.1 RELATED DOCUMENTS A. Drawings and general provisions of the Contract, including General and Supplementary Conditions and Division 1 Specification
THE TRUTH ABOUT TILE & GROUT You re About To Discover The Insider s Secrets to Having Beautiful Tile And Grout BY KEVIN DUCLOS www.britemagic.com TABLE OF CONTENTS Cleaners To Use And Which To Avoid Don
FPD02.qxd 5/18/05 09:37 AM Page 90 2.3 FINISHING PAINTS 2.3.1 INTERIOR AND EXTERIOR METALLIC PAINTS (FORMERLY BRONZE/ALUMINIUM PAINT) Available in a wide range of metallic colours from Silver to Gold e.g.
Extreme Sealing Tape Technical Data May, 2013 Product Description 3M Extreme Sealing Tape is a family of single coated, pressure sensitive adhesive tapes designed for difficult sealing applications. The
How to Build Custom Kitchen Cabinets Submitted by: www.canply.org on October 14, 2011 How to Build Custom Kitchen Cabinets Step by step instructions at the end of this section. Three kitchen cabinets made
Rehabilitation of an Aging Concrete Reservoir Adit Tower Raymond S. Tombaugh, Senior Coatings Consultant KTA-Tator, Inc. and Mongkol Mahavongtrakul, P.E. Corrosion Control Contract Manager San Francisco
SECTION 09900 - PAINTING Contract drawings, Division 0, Conditions of the Contract, and Division1, General Requirements, apply to the Work of this Section PART 1 - GENERAL 1.1 SUMMARY A. Provide materials,
PART 1 - GENERAL CLEANING AND RESTORATION OF SECTION 05900-1 1.1 SUMMARY A. Work on this project shall consist of, but is not limited to, the following: 1. Clean and treat all exposed anodized architectural
Application Procedure Characteristics Product Information is a 3-component high solid durable polyurethane topcoat that provides premium gloss and distinctness of image (DOI) designed to meet and exceed
Metal Preparation Prior to Painting Phosphate 101 - The Basics Doug Van Duyne Metal Pretreatment Paint does not adhere to dirty surfaces Utilizing controlled chemical attack, metal surfaces can be enhanced
SEE HOW TO MAKE LIME PLASTER PATTI STOUTER, BUILD SIMPLE INC. FEBRUARY 2013 WHY USE LIME? Lime plaster forms a light, clean, and durable surface that is resistant to weather and mold. A thin layer attaches
Alkyd performance. Water cleanup. Beckosol AQ is a new platform of low VOC alkyd latex resins made from renewable resources. We take conventional alkyd chemistry and emulsify it in water to deliver a unique
Spraytek Acrylic FAQ s Question: What is the Concrete Coatings, Inc. SprayTek System? Answer: Concrete Coatings Incorporated Spray Tek Acrylic System is a combination of a modified acrylic resin and specially
SIDER-CRETE, INC. 153 Regur Road Hawkinsville, GA 31036 USA Ph: 478.892.9800 www.sider-crete.com MONOBASE RU/ SIDER-PLAST FINISH THE ULTIMATE HARD-COAT/ACRYLIC FINISH SYSTEM 1.0 DESCRIPTION 1.1 General
Brief description The Wecryl waterproofing system allows a high-quality, seamless and crack-bridging waterproofing layer to be installed under loose-laid or bonded surfacing supplied by others (stone slabs,
Rapid Set Products Product Information Product Name: RAPID SET CEMENT ALL 55 LB CONCRETE REPAIR MATERIAL Rapid Set Cement All is a high quality, durable, easy-to-use, multi-purpose repair material that
BEST PRACTICES FOR SOLVENT WELDING THERMOPLASTIC PIPING: PVC, CPVC, and ABS By Stephen Gardiner, IPS Corporation SUMMARY OF PRACTICE MATERIAL PREPARATION SOLVENT WELDING PROCEDURES FOR PLASTIC PIPE AND